Citation Information :
Qaraghuli AM, Signore A, Benedicenti S, El Halawani MT, Solimei L. Comparison and Effect of Common Beverages on Color Stability of Different Esthetic Restorative Materials: An In Vitro Study. J Contemp Dent Pract 2022; 23 (11):1085-1090.
Aim: The aim of this in vitro study is to assess the color stability of different esthetic veneer restorative materials (feldspathic ceramic, hybrid ceramic, zirconia-reinforced lithium silicate glass ceramic, and composite resin) after being exposed to commonly consumed beverages that have staining potential.
Materials and methods: Sixty specimens were prepared into rectangular blocks with fixed dimensions of 10 × 12 × 2.5 mm. Machinable feldspathic ceramic (FC), zirconia-reinforced lithium silicate glass ceramic (LS), and a hybrid ceramic (HC) were milled using CAD/CAM (n = 15), and specimens of microparticle composite resin (MPC) were manually prepared by with the same dimensions (n = 15). All specimens were randomly divided into three subgroups (= 5) according to immersing solutions used (coffee, black tea, and red wine). All specimens were immersed for a period of 72 hours. A colorimetric evaluation was done for each specimen before and after immersion using a spectrophotometer and the difference in color was calculated according to the CIE-Lab system.
To analyze the data, two-way ANOVA and one-way ANOVA tests of significance were used to compare between the different study groups, followed by pairwise comparisons using post hoc test (Tukey).
Results: Different restorative materials showed statistical significance regarding color change after staining (p < 0.001); however, no statistical significance in color change (p > 0.05) was found between the different beverages used.
Conclusion: All tested ceramic materials had better color stability compared with composite resin. All the staining beverages used in the current study might cause a significant color change in the tested restorative materials.
Clinical significance: The color stability of esthetic restorative materials affects their clinical performance in the oral cavity, where the restorative materials are usually exposed to staining beverages that are frequently consumed by patients. Therefore, it is important to understand the staining effect of the different beverages on esthetic restorative materials.
de Oliveira ALBM, Botta AC, Campos JÁDB, et al. Effects of immersion media and repolishing on color stability and superficial morphology of nanofilled composite resin. Microsc Microanal 2014;20(4): 1234–1239. DOI: 10.1017/S1431927614001299.
Fontes ST, Fernández MR, de Moura CM, et al. Color stability of a nanofill composite: Effect of different immersion media. J Appl Oral Sci 2009;17(5):388–391. DOI: 10.1590/s1678-77572009000500007.
Arocha MA, Basilio J, Llopis J, et al. Colour stainability of indirect CAD-CAM processed composites vs conventionally laboratory processed composites after immersion in staining solutions. J Dent 2014;42(7):831–838. DOI: 10.1016/j.jdent.2014.04.002.
Gawriołek M, Sikorska E, Ferreira LF V, et al. Color and luminescence stability of selected dental materials in vitro. J Prosthodont 2012; 21(2):112–122. DOI: 10.1111/j.1532-849X.2011.00808.x.
Davidson SL. Principles of Color Technology, 2nd ed., by Fred W Billmeyer, Jr, and Max Saltzman. Wiley-Interscience, New York, 1981, 240 pp. Color Res Appl 1982;7(3):275–276.
Motro PFK, Kursoglu P, Kazazoglu E. Effects of different surface treatments on stainability of ceramics. J Prosthet Dent 2012;108(4): 231–237. DOI: 10.1016/S0022-3913(12)60168-1.
O'Brien WJ, Groh CL, Boenke KM. A new, small-color-difference equation for dental shades. J Dent Res 1990;69(11):1762–1764. DOI: 10.1177/00220345900690111001.
Goldstein GR, Schmitt GW. Repeatability of a specially designed intraoral colorimeter. J Prosthet Dent 1993;69(6):616–619. DOI: 10.1016/0022-3913(93)90292-v.
Palla ES, Kontonasaki E, Kantiranis N, et al. Color stability of lithium disilicate ceramics after aging and immersion in common beverages. J Prosthet Dent 2018;119(4):632–642. DOI: 10.1016/j.prosdent.2017.04.031.
Johnston WM, Kao EC. Assessment of appearance match by visual observation and clinical colorimetry. J Dent Res 1989;68(5):819–822. DOI: 10.1177/00220345890680051301.
Paravina RD, Swift EJ. Color in dentistry: Match me, match me not. J Esthet Restor Dent 2009;21(2):133–139. DOI: 10.1111/j.1708-8240. 2009.00246.x.
Cengiz S, Yüzbaşioğlu E, Cengiz MI, et al. Color stability and surface roughness of a laboratory-processed composite resin as a function of mouthrinse. J Esthet Restor Dent 2015;27(5):314–321. DOI: 10.1111/jerd.12167.
Dietschi D, Campanile G, Holz J, et al. Comparison of the color stability of ten new-generation composites: An in vitro study. Dent Mater 1994;10(6):353–362. DOI: 10.1016/0109-5641(94)90059-0.
Acar O, Yilmaz B, Altintas SH, et al. Color stainability of CAD/CAM and nanocomposite resin materials. J Prosthet Dent 2016;115(1):71–75. DOI: 10.1016/j.prosdent.2015.06.014.
Ertas E, Guler AU, Yucel AC, et al. Color stability of resin composites after immersion in different drinks. Dent Mater J 2006;25(2):371–376. PMID: 16916243.
Joiner A. Tooth colour: A review of the literature. J Dent 2004;32 (Suppl 1):3–12. DOI: 10.1016/j.jdent.2003.10.013.
Samra APB, Pereira SK, Delgado LC, et al. Color stability evaluation of aesthetic restorative materials. Braz Oral Res 2008;22(3):205–210. DOI: 10.1590/s1806-83242008000300003.
Ghahramanloo A, Madani AS, Sohrabi K, et al. An evaluation of color stability of reinforced composite resin compared with dental porcelain in commonly consumed beverages. J Calif Dent Assoc 2008; 36(9):673–680. PMID: 18856169.
Saygili G, Şahmali S, Demirel F. Colour stability of porcelain repair materials with accelerated ageing. J Oral Rehabil 2006;33(5):387–392. DOI: 10.1111/j.1365-2842.2005.01409.x.
Macentee M, Lakowski R. Instrumental colour measurement of vital and extracted human teeth. J Oral Rehabil 1981;8(3):203–208. DOI: 10.1111/j.1365-2842.1981.tb00494.x.
Ertan AA, Sahin E. Colour stability of low fusing porcelains: An in vitro study. J Oral Rehabil 2005;32(5):358–361. DOI: 10.1111/j.1365-2842.2004.01415.x.
Ayaz EA, Bagis B, Turgut S. Effect of antiasthmatic medication on the surface roughness and color stability of dental restorative materials. Med Princ Pract 2014;23(1):24–28. DOI: 10.1159/000354297.
Ghinea R, Pérez MM, Herrera LJ, et al. Color difference thresholds in dental ceramics. J Dent 2010;38(Suppl 2):e57–e64. DOI: 10.1016/j.jdent.2010.07.008.
Belli R, Geinzer E, Muschweck A, et al. Mechanical fatigue degradation of ceramics versus resin composites for dental restorations. Dent Mater 2014;30(4):424–432. DOI: 10.1016/j.dental.2014.01.003.
Vasudeva G. Monomer systems for dental composites and their future: A review. J Calif Dent Assoc 2009;37(6):389–398. PMID: 19831015.
Guler AU, Yilmaz F, Kulunk T, et al. Effects of different drinks on stainability of resin composite provisional restorative materials. J Prosthet Dent 2005;94(2):118–124. DOI: 10.1016/j.prosdent.2005.05.004.
Poggio C, Ceci M, Beltrami R, et al. Color stability of esthetic restorative materials: A spectrophotometric analysis. Acta Biomater Odontol Scand 2016;2(1):95–101. DOI: 10.1080/23337931.2016.1217416.
Türkün LS, Türkün M. Effect of bleaching and repolishing procedures on coffee and tea stain removal from three anterior composite veneering materials. J Esthet Restor Dent 2004;16(5):290–301. DOI: 10.1111/j.1708-8240.2004.tb00056.x.